J. Phys. Chem. A 2007, 111, 2783-2789
Theoretical Investigation of Electron Paramagnetic Resonance Spectra and Local Structure Distortion for Mn2+ Ions in CaCO3:Mn2+ System: A Simple Model for Mn2+ Ions in a Trigonal Ligand Field Lu Cheng,,† Kuang Xiao-Yu,*,†,‡ Tan Xiao-Ming,† and Yang Xiong† Institute of Atomic and Molecular Physics, Sichuan UniVersity, Chengdu 610065, China, and International Centre for Materials Physics, Academia Sinica, Shenyang 110016, China ReceiVed: October 31, 2006; In Final Form: January 14, 2007
This paper reports on a novel application of a ligand field model for the detection of the local molecular structure of a coordination complex. By diagonalizing the complete energy matrices of the electron-electron repulsion, the ligand field and the spin-orbit coupling for the d5 configuration ion in a trigonal ligand field, the local distortion structure of the (MnO6)10- coordination complex for Mn2+ ions doped into CaCO3, have been investigated. Both the second-order zero-field splitting parameter b02 and the fourth-order zero-field splitting parameter b04 are taken simultaneously in the structural investigation. From the electron paramagnetic resonance (EPR) calculations, the local structure distortion, ∆R ) -0.169 Å to -0.156 Å, ∆θ ) 0.996° to 1.035° for Mn2+ ions in calcite single crystal, ∆R ) -0.185 Å to -0.171 Å, ∆θ ) 3.139° to 3.184° for Mn2+ ions in travertines, and ∆R ) -0.149 Å to -0.102 Å, ∆θ ) 0.791° to 3.927° for Mn2+ ions in shells are determined, respectively. These results elucidate a microscopic origin of various ligand field parameters which are usually used empirically for the interpretation of EPR and optical absorption experiments. It is found that the theoretical results of the EPR and optical absorption spectra for Mn2+ ions in CaCO3 are in good agreement with the experimental findings. Moreover, to understand the detailed physical and chemical properties of the doped CaCO3, the theoretical values of the fourth-order zero-field splitting parameters b04 for Mn2+ ions in travertines and shells are reported first.
I. Introduction Impurities in solid materials have been a subject of widespread interest in recent years as doped materials can display new properties which are absent in pure compounds.1,2 Among the impurities, particular attention has been focused on the transition-metal ions.3-6 The transition-metal divalent manganese ion is perhaps the most investigated impurity ion because the shell of 3d electrons responsible for the paramagnetism is just half filled by the five electrons, and the resultant orbital angular momentum is 0.4-6 Since the total spin is 5/2, it exhibits an additional interaction, the zero-field splitting, and this splitting is highly sensitive to the local structure of manganese centers. Electron paramagnetic resonance (EPR) is regarded as an effective tool to study the microstructure and the local environment around a substitution magnetic ion site in crystals.7,8 The reason is that the EPR spectra usually provide highly detailed microscopic information about the structure of the defects. The EPR spectrum of the Mn2+ paramagnetic ions was used to study the local structure distortions,9 the structural phase transitions,10,11 the existence of a high-spin to low-spin transition,12 and the radicals produced during reaction processes in proteins13 and other biomacromolecules.14-18 So, we can study the local environments of Mn2+ ions from their EPR data. The EPR spectra of transition-metal Mn2+ ions doped into CaCO3 have been experimentally observed by many researchers.19-25 These experimental results give important information about the ground state of the transition-metal Mn2+ ions and * Corresponding author. E-mail: [email protected]
† Sichuan University. ‡ Academia Sinica.
form a useful starting point for understanding the interrelationships between electronic and molecular structure of Mn2+ ions in the (MnO6)10- coordination complex. However, so far, there has been no systematical theory for their analysis. The reason why the previous theoretical results are not quite in good agreement with the observed values may be due to the oversimplification of the theoretical method. For instance, Zheng26 has theoretically investigated the CaCO3:Mn2+ system in single crystal by the superposition model. But in Zheng’s work,26 the calculations of the zero-field splitting parameters b02 and b04 are not in good agreement with the experiment values, which may be ascribed to the fact that the approximate formulas R ≈ (RH + RP)/2 and θ ≈ (θH + θP)/2 were taken in the structural investigation. According to the point-charge model and the superposition model, Yu and Zhao have made a theoretical investigation of the second-order zero-field splitting parameter b02 for Mn2+ ions in the CaCO3:Mn2+ system by using the fourth-order and the sixth-order perturbation formulas.27 However, they did not investigate the fourth-order zerofield splitting parameters b04 of Mn2+ ions in the CaCO3:Mn2+ system. It is well-known that for a d5 configuration ion in a trigonal ligand field, the high-spin ground state is the 6A1 state. To describe the 6A1 ground-state splitting of the Mn2+ ions in the CaCO3:Mn2+ system, the spin Hamiltonian should include three different zero-field splitting parameters b02, b04, and b34. The parameter b34 relates to a fourth-order spin operator and represents a cubic component of the crystalline electric field. The parameters b02 and b04 are respectively associated with the second-order and fourth-order spin operators and represent an
10.1021/jp067161v CCC: $37.00 © 2007 American Chemical Society Published on Web 03/09/2007
2784 J. Phys. Chem. A, Vol. 111, No. 14, 2007
Cheng et al.
Figure 1. Splitting of the energy levels for the Mn2+ ion in the crystal field of trigonal symmetry. a is the cubic field splitting parameter, ∆E1 ) (1/3[(18b02 - 3b04)2 + 9/10(b34)2]1/2 and ∆E2 ) -b02 - (9/2)b04 ( 1/6[(18b02 - 3b04)2 + 9/10(b34)2]1/2 are the zero-field splitting energies in the ground state 6A1. The positive and negative signs correspond to b02 g 0 and b02 < 0, respectively.32
axial component of the crystalline electric field that is axially symmetric about the C3 axis. In order to explain more reasonably structure distortion, herein, we suggest that the two zero-field splitting parameters b02 and b04 should be simultaneously considered in the determination of the local structure distortion of Mn2+ ions in the CaCO3:Mn2+ system. In the present work, a theoretical model for determining the local structure distortion of Mn2+ ions in the (MnO6)10- coordination complex is proposed by diagonalizing the complete energy matrices for the d5 configuration ion in a trigonal ligand field and by considering the second-order and fourth-order zero-field splitting parameters b02 and b04 simultaneously. By this model, the optical absorption and EPR spectra of Mn2+ ions in calcite single crystal, travertines and shells have been investigated. II. Ligand Field Model Firstly, we construct the complete energy matrix of the d5 configuration ion within the ligand field scheme. There are two different ways which have been developed to construct the complete matrix. One way is Racah’s method, in which the tensor operator has been used;28 the other way is Slater’s method, in which the relationships between the matrix of the single d electron and the matrix of the dn configuration have been established.29 In the present work, Slater’s method has been employed. For a d5 configuration ion in a trigonal ligand field, in order to construct the complete matrixes, the |J,MJ〉 basic functions need to expand into the form of the |L,S,ML,MS〉i basic functions. This expansion may be realized in terms of the
Clebsch-Gordon coefficients which are associated with the coupling of two angular moments. In general, the expansion can be written as30
∑ (j1j2m1m2||j1j2jm)ψj m ψj m ) m∑m
(2j + 1)
(j + j1 - j2)!(j - j1 + j2)!(j1 + j2 - j)! (j + j1 + j2 + 1)!
× (j1 + m1)!
(j1 - m1)!(j2 + m2)!(j2 - m2)!(j + m)!(j - m)!
(- 1)γ [(j1 + j2 - j - γ)!(j1 - m1 - γ)!(j2 + m2 - γ)! × γ!
(j - j2 + m1 + γ)!(j - j1 - m2 + γ)!]-1 ψj1m1ψj2m2 (1) The relationship of the coefficients between m and -m is
〈j1j2m1m2||j1j2jm〉 ) (- 1)j1+j2-j〈j1j2 - m1 - m2||j1j2j - m〉 (2) From eqs 1 and 2, it is easy to get the |J,MJ〉 basic functions
∑i Ci|L,S,ML,MS〉i ) ∑i ∑j CiCjΦj
Model for Mn2+ Ions in a Trigonal Ligand Field
J. Phys. Chem. A, Vol. 111, No. 14, 2007 2785
Figure 2. (1) Rhombohedral unit cell of calcite. (2) Local structure distortion for Mn2+ ions in the CaCO3:Mn2+ system. R0 and θ0 are the structure parameters of CaCO3. ∆R and ∆θ represent the structure distortion. R is the Mn-O bond lengths. θ is the angle between the Mn-O bond and the C3 axis when the Mn2+ ion replaces the Ca2+ ion.
where Ci and Cj are the Clebsch-Gordon coefficients and Φj is one of the 252 basic Slater determinants. According to the |L,S,ML,MS〉i functions of the d5 configuration ion in a trigonal ligand field, we have constructed the complete energy matrix of the Hamiltonian
H ˆ )H ˆ ee + H ˆ so + H ˆ lf )
∑ i 0. This compressed distortion may be attributed to the fact that the Mn2+ ion has an obviously smaller ionic radius ( rMn2+ ) 0.91 Å) than that of the Ca2+ ion ( rCa2+ ) 1.00 Å).52 It should be also noted that the local lattice structure of the CaCO3:Mn2+ system in travertines and shells are obviously different from those in calcite single crystal. This result may be explained by the external environmental factor, such as the density of the Mn2+ ions in water and the temperature of the
2788 J. Phys. Chem. A, Vol. 111, No. 14, 2007 water. Of course, other factors can also affect the local structure, such as deposition and infiltration of clay minerals, dissolution and recrystallization cycles of CaCO3, impurity of the protein and mucopolysaccharides, and biological action. Using the complete diagonalization method, we establish the inter-relationships between electronic and molecular structure and study the local molecular structure of the (MnO6)10coordination complex. By comparing our theoretical results (R ) 2.191-2.204 Å, θ ) 53.796-53.853°) with the results (R ) 2.29 Å, θ ) 53.46°) obtained by Zheng,26 we find it noteworthy to mention that the empirical formulas R ≈ (RH + RP)/2 and θ ≈ (θH + θP)/2 are not suitable for the CaCO3:Mn2+ system. Furthermore, the previous theoretical result of the second-order zero-field splitting parameter b02 (b02 ) -82 × 10-4 cm-1) obtained by Yu and Zhao27 is not quite in good agreement with the observed value (b02 ) -75.96 × 10-4 cm-1) for Mn2+ ions in the CaCO3:Mn2+ system.24 This indicates that the high-order perturbation method is imperfect. Considering that the two zerofield splitting parameters are useful in understanding the coupling strength of Mn2+ ions to the CaCO3 lattice and accordingly in understanding the changes of other properties induced by the Mn2+ impurity, we have constructed the complete energy matrixes for d5 configuration ion in a trigonal ligand field and have made an analysis of the zero-field splitting parameters b02 and b04 of Mn2+ ions in the CaCO3:Mn2+ system. This is a generic theoretical method. It is very interesting as the complete diagonalization method avoids perturbation solutions which are known to be extremely sensitive to the part of the matrix included in the determination of relationships between the crystal field and the spin Hamiltonian parameters. At the same time, this theoretical method opens the possibilities to test a different approximate method, for example, the high-order perturbation method. Of course, our theoretical results remain to be checked by other more direct experiments.
Cheng et al. Acknowledgment. The authors express their gratitude to Dr. Zhu Ben-Chao for many helpful discussions. This work was supported by the National Natural Science Foundation (No. 10374068) and the Doctoral Education Fund of Education Ministry (No. 20050610011) of China. Appendix Ligand Field Potential. The ligand field potential Vi in eq 4 can be written as53
Vi ) γ00Z00 + γ20ri2Z20(θi, φi) + γ40ri4Z40(θi, φi) + γc43ri4Zc43 (θi, φi) + γs43ri4Zs43(θi, φi) where ri, θi, and φi are spherical coordinates of the ith electron. Zlm, Zclm and Zslm are defined as
Zl0 ) Yl0 Zclm ) (1/x2)[Yl,-m + (- 1)mYl,m] Zslm ) (i/x2)[Yl,-m - (- 1)mYl,m] The Yl,m are the spherical harmonics. γl0, γclm, and γslm are associated with the local lattice structure around the d5 configuration ion by the relations
γl0 ) -
γclm ) -
∑ 2l + 1τ)1
2l + 1τ)1Rl+1
IV. Conclusion From the above studies, we have the following conclusions. (i) The EPR and optical absorption spectra of Mn2+ ions in CaCO3 have been studied by the complete energy matrices for a d5 configuration ion in a trigonal ligand field. It is worth noting that the above theoretical study of EPR and optical absorption spectra provides powerful guidelines for future experimental studies aimed at pinpointing exactly how Mn enters into the CaCO3 environment. (ii) By solving the energy matrices, the zero-field splitting parameters b02 and b04 have been derived, and the theoretical values are found to be in good agreement with the experimental findings. (iii) From the EPR calculation, local structure distortion parameters ∆R and ∆θ for Mn2+ ions in CaCO3 are determined. The results show that the local lattice structure of the (MnO6)10coordination complex for Mn2+ ions in the CaCO3:Mn2+ system has a compressed distortion and the local lattice structure of the CaCO3:Mn2+ system for Mn2+ ions in travertines and shells are obviously different from those in calcite single crystal. Moreover, the theoretical values of the zero-field splitting parameter b04 for Mn2+ ions in travertines and shells are reported first. These parameters are of significance in broadening our understanding of the physical and chemical properties of CaCO3. Of course, careful experimental investigations, especially electron nuclear double resonance (ENDOR) experiments, are required in order to clarify the local structure around the Mn2+ ions in the CaCO3:Mn2+ system in detail.
∑ 2l + 1τ)1
where θτ and φτ are angular coordinates of the ligand. τ and qτ represent the τth ligand ion and its effective charge, respectively. Rτ denotes the impurity-ligand distance. References and Notes (1) Misra, S. K.; Andronenko, S. I. J. Phys. Chem. B 2004, 108, 9397. (2) Zhecheva, E.; Stoyanova, R.; Alca´ntara, R.; Tirado, J. L. J. Phys. Chem. B 2003, 107, 4290. (3) Jeschke, G. J. Phys. Chem. B 2000, 104, 8382. (4) Mantel, C.; Baffert, C.; Romero, I.; Deronzier, A.; Pe´caut, J.; Collomb, M. N.; Duboc, C. Inorg. Chem. 2004, 43, 6455. (5) Dasgupta, J.; Tyryshkin, A. M.; Kozlov, Y. N.; Klimov, V. V.; Dismukes, G. C. J. Phys. Chem. B 2006, 110, 5099. (6) Zong, X. H.; Zhou, P.; Shao, Z. Z.; Chen, S. M.; Chen, X.; Hu, B. W.; Deng, F.; Yao, W. H. Biochemistry 2004, 43, 11932. (7) Keeble, D. J.; Loyo-Menoyo, M.; Furukawa, Y.; Kitamura, K. Phys. ReV. B: Condens. Matter Mater. Phys. 2005, 71, 224111. (8) Diaconu, M.; Schmidt, H.; Po¨ppl, A.; Bo¨ttcher, R.; Hoentsch, J.; Klunker, A.; Spemann, D.; Hochmuth, H.; Lorenz, M.; Grundmann, M. Phys. ReV. B: Condens. Matter Mater. Phys. 2005, 72, 085214. (9) Caudle, M. T.; Mobley, C. K.; Bafaro, L. M.; LoBrutto, R.; Yee, G. T.; Groy, T. L. Inorg. Chem. 2004, 43, 506. (10) Zapart, W. J. Phys. Chem. B 2003, 107, 4208. (11) Augustyniak-Jabłokow, M. A.; Krupska, A.; Krupski, M.; Yablokov, Y. V. Inorg. Chem. 2002, 41, 1348. (12) Ozarowski, A.; Mcgarvey, B. R.; Sarkar, A. B.; Drake, J. E. Inorg. Chem. 1988, 27, 628. (13) Smirnova, T. I.; Smirnov, A. I. J. Phys. Chem. B 2003, 107, 7212. (14) Renault, J. P.; Verche`re-Be´aur, C.; Morgenstern-Badarau, I.; Yamakura, F.; Gerloch, M. Inorg. Chem. 2000, 39, 2666.
Model for Mn2+ Ions in a Trigonal Ligand Field (15) Duboc-Toia, C.; Hassan, A. K.; Mulliez, E.; Ollagnier-de Choudens, S.; Fontecave, M.; Leutwein, C.; Heider, J. J. Am. Chem. Soc. 2003, 125, 38. (16) Mantel, C.; Hassan, A. K.; Pe´caut, J.; Deronzier, A.; Collomb, M. N.; Duboc-Toia, C. J. Am. Chem. Soc. 2003, 125, 12337. (17) Wilson, J. C.; Wu, G.; Tsai, A.; Gerfen, G. J. J. Am. Chem. Soc. 2005, 127, 1618. (18) Bertholon, I.; Hommel, H.; Labarre, D.; Vauthier, C. Langmuir 2006, 22, 5485. (19) Benedetto, F. D.; Montegrossi, G.; Pardi, L. A.; Minissale, A.; Paladini, M.; Romanelli, M. J. Magn. Reson. 2005, 177, 86. (20) Montegrossi, G.; Di Benedetto, F.; Minissale, A.; Paladini, M.; Pardi, L. A.; Romanelli, M.; Romei, F. Appl. Geochem. 2006, 21, 820. (21) Barberis, G. E.; Calvo, R.; Maldonado, H. G.; Zarate, C. E. Phys. ReV. B: Condens. Matter Mater. Phys. 1975, 12, 853. (22) Serway, R. A. Phys. ReV. B: Condens. Matter Mater. Phys. 1971, 3, 608. (23) Wait, D. F. Phys. ReV. 1963, 132, 601. (24) Slezak, A.; Lech, J.; Bojko, I. Phys. Status Solidi A 1979, 54, 755. (25) Tennant, W. C. J. Magn. Reson. 1974, 14, 152. (26) Zheng, W. C. Physica B (Amsterdam, Neth.) 1997, 240, 211. (27) Yu, W. L.; Zhao, M. G. J. Phys. C: Solid State Phys. 1987, 20, 4647. (28) Griffith, J. S. The Theory of Transition-Metal Ions; Cambridge University Press: London, 1964. (29) Slater, J. C. Quantum Theory of Molecules and Solids; McGrawHill, New York, 1963; Vol. I. (30) Zare, R. N. Angular Momentum; John Wiley & Sons: New York, 1988. (31) Newman, D. J.; Urban, W. AdV. Phys. 1975, 24, 793. (32) Abragam, A.; Bleaney, B. Electron Paramagnetic Resonance of Transition Ions; Clarendon Press: Oxford, 1970.
J. Phys. Chem. A, Vol. 111, No. 14, 2007 2789 (33) Stevens, K. W. H. Proc. Phys. Soc., London 1952, 65, 209. (34) Marshall, S. A.; Serway, R. A. Phys. ReV. 1968, 171, 345. (35) Garribba, E.; Micera, G. Magn. Reson. Chem. 2006, 44, 11. (36) Newman, D. J.; Ng, B. Rep. Prog. Phys. 1989, 52, 699. (37) Vleck, J. H. V. Phys. ReV. 1932, 41, 208. (38) Zhao, M. G.; Bai, G. R.; Jin, H. C. J. Phys. C: Solid State Phys. 1982, 15, 5959. (39) L. L. L., Jr. J. Chem. Phys. 1966, 45, 3611. (40) Cheng, L.; Sturchio, N. C.; Bedzyk, M. J. Phys. ReV. B: Condens. Matter Mater. Phys. 2001, 63, 144104. (41) Pappalardo, R. J. Chem. Phys. 1960, 33, 613. (42) Van, E. W.; Haas, C. Phys. Status Solidi B 1975, 70, 517. (43) Ronda, C. R.; Siekman, H. H.; Haas, C. Physica B 1987, 144, 331. (44) Newman, D. J.; Siegel, E. J. Phys. C: Solid State Phys. 1976, 9, 4285. (45) Curie, D.; Barthon, C.; Canny, B. J. Chem. Phys. 1974, 61, 3048. (46) Kuang, X. Y.; Zhang, W.; Morgenstern-Badarau, I. Phys. ReV. B: Condens. Matter Mater. Phys. 1992, 45, 8104. (47) Blanchard, S. C.; Chasteen, N. D. J. Phys. Chem. 1976, 80, 1362. (48) Prasuna, C. P. L.; Narasimhulu, K. V.; Gopal, N. O.; Rao, J. L.; Rao, T. V. R. K. Spectrochim. Acta. A 2004, 60, 2305. (49) Narasimhulu, K. V.; Rao, J. L. Spectrochim. Acta, Part A 2000, 56, 1345. (50) Raju, C. L.; Narasimhulu, K. V.; Gopal, N. O.; Rao, J. L.; Reddy, B. C. V. J. Mol. Struct. 2002, 608, 201. (51) Naidu, Y. N.; Rao, J. L.; Lakshman, S. V. J. Polyhedron 1992, 11, 663. (52) Polikreti, K.; Maniatis, Y. Atmos. EnViron. 2004, 38, 3617. (53) Hutchings, M. T. Solid State Phys. 1964, 16, 227.